 
data_1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'Ba F2 Mo2 O10 Te2' 
_chemical_formula_weight          782.41 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'Ba'  'Ba'  -0.3244   2.2819 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'F'  'F'   0.0171   0.0103 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Te'  'Te'  -0.5308   1.6751 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            orthorhombic 
_symmetry_space_group_name_H-M    Aba2 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, z' 
 '-x+1/2, y, z+1/2' 
 'x+1/2, -y, z+1/2' 
 'x, y+1/2, z+1/2' 
 '-x, -y+1/2, z+1/2' 
 '-x+1/2, y+1/2, z+1' 
 'x+1/2, -y+1/2, z+1' 
 
_cell_length_a                    12.5591(14) 
_cell_length_b                    11.0137(9) 
_cell_length_c                    7.2753(8) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.00 
_cell_angle_gamma                 90.00 
_cell_volume                      1006.34(18) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     1661 
_cell_measurement_theta_min       3.2443 
_cell_measurement_theta_max       27.1203 
 
_exptl_crystal_description        rod-like 
_exptl_crystal_colour             colorless 
_exptl_crystal_size_max           0.16 
_exptl_crystal_size_mid           0.07 
_exptl_crystal_size_min           0.06 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     5.164 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1368 
_exptl_absorpt_coefficient_mu     12.083 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.4375 
_exptl_absorpt_correction_T_max   0.7455 
_exptl_absorpt_process_details    'SADABS V2014/5 (Bruker AXS Inc.)'
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   bruker-CCD 
_diffrn_measurement_method        'w scans'
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             2500 
_diffrn_reflns_av_R_equivalents   0.0305 
_diffrn_reflns_av_sigmaI/netI     0.0407 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        16 
_diffrn_reflns_limit_k_min        -14 
_diffrn_reflns_limit_k_max        12 
_diffrn_reflns_limit_l_min        -8 
_diffrn_reflns_limit_l_max        9 
_diffrn_reflns_theta_min          3.24 
_diffrn_reflns_theta_max          27.12 
_reflns_number_total              1015 
_reflns_number_gt                 936 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'Bruker APEX2'
_computing_cell_refinement        'Bruker SAINT' 
_computing_data_reduction         'Bruker SAINT'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0120P)²+49.8492P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    none 
_refine_ls_hydrogen_treatment     none 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00163(16) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_abs_structure_details 
 'Flack H D (1983), Acta Cryst. A39, 876-881' 
_refine_ls_abs_structure_Flack    0.00 
_refine_ls_number_reflns          1015 
_refine_ls_number_parameters      88 
_refine_ls_number_restraints      37 
_refine_ls_R_factor_all           0.0358 
_refine_ls_R_factor_gt            0.0297 
_refine_ls_wR_factor_ref          0.0856 
_refine_ls_wR_factor_gt           0.0643 
_refine_ls_goodness_of_fit_ref    1.196 
_refine_ls_restrained_S_all       1.181 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Mo1 Mo 0.11671(6) 0.17467(7) 0.1554(3) 0.0064(3) Uani 1 1 d . . . 
F1 F 0.3580(10) 0.3282(13) -0.1728(15) 0.023(3) Uani 1 1 d . . . 
O1 O 0.2734(6) 0.1787(7) 0.163(2) 0.0164(17) Uani 1 1 d U . . 
O2 O 0.1046(9) 0.0739(12) -0.0267(17) 0.008(3) Uani 1 1 d U . . 
O3 O 0.4727(5) 0.2577(7) 0.160(2) 0.0116(15) Uani 1 1 d U . . 
O4 O 0.0969(10) 0.0809(12) 0.3373(19) 0.015(3) Uani 1 1 d U . . 
O5 O 0.1424(11) 0.3332(14) -0.0247(16) 0.011(2) Uani 1 1 d U . . 
Te1 Te 0.33896(15) 0.33053(17) 0.21157(10) 0.0100(3) Uani 0.70 1 d P . . 
Te1A Te 0.3382(3) 0.3317(4) 0.0976(4) 0.0028(6) Uani 0.30 1 d PU . . 
Ba1 Ba 0.0000 0.0000 0.6572(4) 0.0105(3) Uani 1 2 d S . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Mo1 O4 1.697(14) . ? 
Mo1 O2 1.735(12) . ? 
Mo1 O3 1.956(7) 8_454 ? 
Mo1 O1 1.970(8) . ? 
Mo1 F1 2.127(13) 3 ? 
Mo1 O5 2.207(15) . ? 
Mo1 Te1A 3.302(4) . ? 
Mo1 Te1 3.302(2) . ? 
F1 Te1A 1.984(12) . ? 
F1 Mo1 2.127(13) 3_554 ? 
F1 Te1 2.613(13) 3_554 ? 
O1 Te1 1.897(8) . ? 
O1 Te1A 1.930(9) . ? 
O3 Te1 1.899(8) . ? 
O3 Te1A 1.930(9) . ? 
O3 Mo1 1.956(7) 8_554 ? 
O5 Te1 1.933(12) 3_554 ? 
O5 Te1A 2.615(14) . ? 
Te1 Te1A 0.829(3) . ? 
Te1 O5 1.933(12) 3 ? 
Te1 F1 2.613(13) 3 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O4 Mo1 O2 101.1(3) . . ? 
O4 Mo1 O3 94.7(6) . 8_454 ? 
O2 Mo1 O3 100.2(5) . 8_454 ? 
O4 Mo1 O1 98.0(6) . . ? 
O2 Mo1 O1 97.1(5) . . ? 
O3 Mo1 O1 156.2(3) 8_454 . ? 
O4 Mo1 F1 92.7(6) . 3 ? 
O2 Mo1 F1 166.1(5) . 3 ? 
O3 Mo1 F1 79.9(5) 8_454 3 ? 
O1 Mo1 F1 79.4(5) . 3 ? 
O4 Mo1 O5 165.0(6) . . ? 
O2 Mo1 O5 93.8(5) . . ? 
O3 Mo1 O5 81.0(5) 8_454 . ? 
O1 Mo1 O5 81.5(5) . . ? 
F1 Mo1 O5 72.4(3) 3 . ? 
O4 Mo1 Te1A 122.8(4) . . ? 
O2 Mo1 Te1A 108.2(4) . . ? 
O3 Mo1 Te1A 125.6(2) 8_454 . ? 
O1 Mo1 Te1A 31.8(3) . . ? 
F1 Mo1 Te1A 62.1(3) 3 . ? 
O5 Mo1 Te1A 52.2(4) . . ? 
O4 Mo1 Te1 110.1(4) . . ? 
O2 Mo1 Te1 120.1(4) . . ? 
O3 Mo1 Te1 125.5(2) 8_454 . ? 
O1 Mo1 Te1 30.7(2) . . ? 
F1 Mo1 Te1 52.2(3) 3 . ? 
O5 Mo1 Te1 62.5(3) . . ? 
Te1A Mo1 Te1 14.42(5) . . ? 
Te1A F1 Mo1 128.1(7) . 3_554 ? 
Te1A F1 Te1 101.6(5) . 3_554 ? 
Mo1 F1 Te1 87.7(4) 3_554 3_554 ? 
Te1 O1 Te1A 25.01(14) . . ? 
Te1 O1 Mo1 117.3(4) . . ? 
Te1A O1 Mo1 115.7(4) . . ? 
Te1 O3 Te1A 24.99(12) . . ? 
Te1 O3 Mo1 131.3(5) . 8_554 ? 
Te1A O3 Mo1 130.1(5) . 8_554 ? 
Te1 O5 Mo1 126.5(7) 3_554 . ? 
Te1 O5 Te1A 102.9(6) 3_554 . ? 
Mo1 O5 Te1A 86.0(4) . . ? 
Te1A Te1 O1 79.7(5) . . ? 
Te1A Te1 O3 79.6(6) . . ? 
O1 Te1 O3 88.5(3) . . ? 
Te1A Te1 O5 173.5(6) . 3 ? 
O1 Te1 O5 104.6(6) . 3 ? 
O3 Te1 O5 95.5(7) . 3 ? 
Te1A Te1 F1 108.1(5) . 3 ? 
O1 Te1 F1 68.9(4) . 3 ? 
O3 Te1 F1 153.7(4) . 3 ? 
O5 Te1 F1 78.2(4) 3 3 ? 
Te1A Te1 Mo1 82.8(4) . . ? 
O1 Te1 Mo1 32.0(2) . . ? 
O3 Te1 Mo1 120.2(3) . . ? 
O5 Te1 Mo1 103.5(4) 3 . ? 
F1 Te1 Mo1 40.1(3) 3 . ? 
Te1 Te1A O1 75.3(5) . . ? 
Te1 Te1A O3 75.4(6) . . ? 
O1 Te1A O3 86.7(4) . . ? 
Te1 Te1A F1 171.9(6) . . ? 
O1 Te1A F1 106.3(6) . . ? 
O3 Te1A F1 96.6(7) . . ? 
Te1 Te1A O5 110.6(5) . . ? 
O1 Te1A O5 72.1(5) . . ? 
O3 Te1A O5 154.9(5) . . ? 
F1 Te1A O5 77.3(4) . . ? 
Te1 Te1A Mo1 82.8(4) . . ? 
O1 Te1A Mo1 32.5(2) . . ? 
O3 Te1A Mo1 119.1(3) . . ? 
F1 Te1A Mo1 102.8(4) . . ? 
O5 Te1A Mo1 41.8(3) . . ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
O4 Mo1 O1 Te1 -116.4(8) . . . . ? 
O2 Mo1 O1 Te1 141.3(8) . . . . ? 
O3 Mo1 O1 Te1 5(2) 8_454 . . . ? 
F1 Mo1 O1 Te1 -25.1(7) 3 . . . ? 
O5 Mo1 O1 Te1 48.5(7) . . . . ? 
Te1A Mo1 O1 Te1 28.0(2) . . . . ? 
O4 Mo1 O1 Te1A -144.3(8) . . . . ? 
O2 Mo1 O1 Te1A 113.3(8) . . . . ? 
O3 Mo1 O1 Te1A -23(2) 8_454 . . . ? 
F1 Mo1 O1 Te1A -53.0(7) 3 . . . ? 
O5 Mo1 O1 Te1A 20.5(7) . . . . ? 
Te1 Mo1 O1 Te1A -28.0(2) . . . . ? 
O4 Mo1 O5 Te1 178.7(17) . . . 3_554 ? 
O2 Mo1 O5 Te1 -6.9(9) . . . 3_554 ? 
O3 Mo1 O5 Te1 -106.6(9) 8_454 . . 3_554 ? 
O1 Mo1 O5 Te1 89.6(9) . . . 3_554 ? 
F1 Mo1 O5 Te1 171.2(12) 3 . . 3_554 ? 
Te1A Mo1 O5 Te1 103.2(9) . . . 3_554 ? 
Te1 Mo1 O5 Te1 115.2(9) . . . 3_554 ? 
O4 Mo1 O5 Te1A 76(2) . . . . ? 
O2 Mo1 O5 Te1A -110.1(5) . . . . ? 
O3 Mo1 O5 Te1A 150.2(5) 8_454 . . . ? 
O1 Mo1 O5 Te1A -13.5(4) . . . . ? 
F1 Mo1 O5 Te1A 68.0(4) 3 . . . ? 
Te1 Mo1 O5 Te1A 11.99(13) . . . . ? 
Mo1 O1 Te1 Te1A -92.8(8) . . . . ? 
Te1A O1 Te1 O3 -79.7(6) . . . . ? 
Mo1 O1 Te1 O3 -172.5(9) . . . . ? 
Te1A O1 Te1 O5 -175.0(6) . . . 3 ? 
Mo1 O1 Te1 O5 92.2(8) . . . 3 ? 
Te1A O1 Te1 F1 114.1(5) . . . 3 ? 
Mo1 O1 Te1 F1 21.3(6) . . . 3 ? 
Te1A O1 Te1 Mo1 92.8(8) . . . . ? 
Mo1 O3 Te1 Te1A 98.3(12) 8_554 . . . ? 
Te1A O3 Te1 O1 79.8(5) . . . . ? 
Mo1 O3 Te1 O1 178.1(12) 8_554 . . . ? 
Te1A O3 Te1 O5 -175.7(6) . . . 3 ? 
Mo1 O3 Te1 O5 -77.4(12) 8_554 . . 3 ? 
Te1A O3 Te1 F1 110.0(12) . . . 3 ? 
Mo1 O3 Te1 F1 -151.7(6) 8_554 . . 3 ? 
Te1A O3 Te1 Mo1 75.2(5) . . . . ? 
Mo1 O3 Te1 Mo1 173.5(8) 8_554 . . . ? 
O4 Mo1 Te1 Te1A 153.1(6) . . . . ? 
O2 Mo1 Te1 Te1A 36.4(6) . . . . ? 
O3 Mo1 Te1 Te1A -95.2(7) 8_454 . . . ? 
O1 Mo1 Te1 Te1A 82.2(9) . . . . ? 
F1 Mo1 Te1 Te1A -129.6(6) 3 . . . ? 
O5 Mo1 Te1 Te1A -41.2(6) . . . . ? 
O4 Mo1 Te1 O1 70.9(10) . . . . ? 
O2 Mo1 Te1 O1 -45.8(10) . . . . ? 
O3 Mo1 Te1 O1 -177.4(10) 8_454 . . . ? 
F1 Mo1 Te1 O1 148.2(9) 3 . . . ? 
O5 Mo1 Te1 O1 -123.4(9) . . . . ? 
Te1A Mo1 Te1 O1 -82.2(9) . . . . ? 
O4 Mo1 Te1 O3 79.6(7) . . . . ? 
O2 Mo1 Te1 O3 -37.1(8) . . . . ? 
O3 Mo1 Te1 O3 -168.7(12) 8_454 . . . ? 
O1 Mo1 Te1 O3 8.7(10) . . . . ? 
F1 Mo1 Te1 O3 156.9(7) 3 . . . ? 
O5 Mo1 Te1 O3 -114.7(7) . . . . ? 
Te1A Mo1 Te1 O3 -73.5(7) . . . . ? 
O4 Mo1 Te1 O5 -25.1(6) . . . 3 ? 
O2 Mo1 Te1 O5 -141.8(6) . . . 3 ? 
O3 Mo1 Te1 O5 86.6(8) 8_454 . . 3 ? 
O1 Mo1 Te1 O5 -96.0(10) . . . 3 ? 
F1 Mo1 Te1 O5 52.2(7) 3 . . 3 ? 
O5 Mo1 Te1 O5 140.6(7) . . . 3 ? 
Te1A Mo1 Te1 O5 -178.1(6) . . . 3 ? 
O4 Mo1 Te1 F1 -77.3(7) . . . 3 ? 
O2 Mo1 Te1 F1 166.0(7) . . . 3 ? 
O3 Mo1 Te1 F1 34.4(8) 8_454 . . 3 ? 
O1 Mo1 Te1 F1 -148.2(9) . . . 3 ? 
O5 Mo1 Te1 F1 88.4(4) . . . 3 ? 
Te1A Mo1 Te1 F1 129.6(6) . . . 3 ? 
O3 Te1 Te1A O1 90.4(3) . . . . ? 
O5 Te1 Te1A O1 132(5) 3 . . . ? 
F1 Te1 Te1A O1 -63.7(4) 3 . . . ? 
Mo1 Te1 Te1A O1 -32.2(2) . . . . ? 
O1 Te1 Te1A O3 -90.4(3) . . . . ? 
O5 Te1 Te1A O3 41(5) 3 . . . ? 
F1 Te1 Te1A O3 -154.1(4) 3 . . . ? 
Mo1 Te1 Te1A O3 -122.6(2) . . . . ? 
O1 Te1 Te1A F1 -102(4) . . . . ? 
O3 Te1 Te1A F1 -11(4) . . . . ? 
O5 Te1 Te1A F1 30(9) 3 . . . ? 
F1 Te1 Te1A F1 -165(4) 3 . . . ? 
Mo1 Te1 Te1A F1 -134(4) . . . . ? 
O1 Te1 Te1A O5 64.0(5) . . . . ? 
O3 Te1 Te1A O5 154.4(5) . . . . ? 
O5 Te1 Te1A O5 -164(6) 3 . . . ? 
F1 Te1 Te1A O5 0.4(8) 3 . . . ? 
Mo1 Te1 Te1A O5 31.8(4) . . . . ? 
O1 Te1 Te1A Mo1 32.2(2) . . . . ? 
O3 Te1 Te1A Mo1 122.6(2) . . . . ? 
O5 Te1 Te1A Mo1 164(5) 3 . . . ? 
F1 Te1 Te1A Mo1 -31.4(4) 3 . . . ? 
Mo1 O1 Te1A Te1 99.9(8) . . . . ? 
Te1 O1 Te1A O3 75.8(6) . . . . ? 
Mo1 O1 Te1A O3 175.7(9) . . . . ? 
Te1 O1 Te1A F1 171.7(7) . . . . ? 
Mo1 O1 Te1A F1 -88.4(8) . . . . ? 
Te1 O1 Te1A O5 -117.8(5) . . . . ? 
Mo1 O1 Te1A O5 -17.9(6) . . . . ? 
Te1 O1 Te1A Mo1 -99.9(8) . . . . ? 
Mo1 O3 Te1A Te1 -103.7(11) 8_554 . . . ? 
Te1 O3 Te1A O1 -75.6(5) . . . . ? 
Mo1 O3 Te1A O1 -179.3(12) 8_554 . . . ? 
Te1 O3 Te1A F1 178.4(6) . . . . ? 
Mo1 O3 Te1A F1 74.7(12) 8_554 . . . ? 
Te1 O3 Te1A O5 -107.5(14) . . . . ? 
Mo1 O3 Te1A O5 148.9(8) 8_554 . . . ? 
Te1 O3 Te1A Mo1 -73.0(5) . . . . ? 
Mo1 O3 Te1A Mo1 -176.6(8) 8_554 . . . ? 
Mo1 F1 Te1A Te1 70(5) 3_554 . . . ? 
Te1 F1 Te1A Te1 167(4) 3_554 . . . ? 
Mo1 F1 Te1A O1 -29.2(9) 3_554 . . . ? 
Te1 F1 Te1A O1 67.0(5) 3_554 . . . ? 
Mo1 F1 Te1A O3 59.3(8) 3_554 . . . ? 
Te1 F1 Te1A O3 155.5(4) 3_554 . . . ? 
Mo1 F1 Te1A O5 -96.1(9) 3_554 . . . ? 
Te1 F1 Te1A O5 0.2(2) 3_554 . . . ? 
Mo1 F1 Te1A Mo1 -62.7(8) 3_554 . . . ? 
Te1 F1 Te1A Mo1 33.6(5) 3_554 . . . ? 
Te1 O5 Te1A Te1 -178.2(6) 3_554 . . . ? 
Mo1 O5 Te1A Te1 -51.6(6) . . . . ? 
Te1 O5 Te1A O1 -112.2(7) 3_554 . . . ? 
Mo1 O5 Te1A O1 14.4(5) . . . . ? 
Te1 O5 Te1A O3 -78.6(16) 3_554 . . . ? 
Mo1 O5 Te1A O3 48.0(15) . . . . ? 
Te1 O5 Te1A F1 -0.2(3) 3_554 . . . ? 
Mo1 O5 Te1A F1 126.3(7) . . . . ? 
Te1 O5 Te1A Mo1 -126.6(8) 3_554 . . . ? 
O4 Mo1 Te1A Te1 -30.4(6) . . . . ? 
O2 Mo1 Te1A Te1 -147.3(5) . . . . ? 
O3 Mo1 Te1A Te1 95.1(7) 8_454 . . . ? 
O1 Mo1 Te1A Te1 -73.8(8) . . . . ? 
F1 Mo1 Te1A Te1 43.5(5) 3 . . . ? 
O5 Mo1 Te1A Te1 132.3(6) . . . . ? 
O4 Mo1 Te1A O1 43.4(10) . . . . ? 
O2 Mo1 Te1A O1 -73.5(9) . . . . ? 
O3 Mo1 Te1A O1 168.9(10) 8_454 . . . ? 
F1 Mo1 Te1A O1 117.3(9) 3 . . . ? 
O5 Mo1 Te1A O1 -153.9(9) . . . . ? 
Te1 Mo1 Te1A O1 73.8(8) . . . . ? 
O4 Mo1 Te1A O3 38.4(8) . . . . ? 
O2 Mo1 Te1A O3 -78.5(7) . . . . ? 
O3 Mo1 Te1A O3 164.0(12) 8_454 . . . ? 
O1 Mo1 Te1A O3 -5.0(10) . . . . ? 
F1 Mo1 Te1A O3 112.4(7) 3 . . . ? 
O5 Mo1 Te1A O3 -158.9(7) . . . . ? 
Te1 Mo1 Te1A O3 68.8(7) . . . . ? 
O4 Mo1 Te1A F1 143.6(6) . . . . ? 
O2 Mo1 Te1A F1 26.7(6) . . . . ? 
O3 Mo1 Te1A F1 -90.8(7) 8_454 . . . ? 
O1 Mo1 Te1A F1 100.2(9) . . . . ? 
F1 Mo1 Te1A F1 -142.4(7) 3 . . . ? 
O5 Mo1 Te1A F1 -53.7(7) . . . . ? 
Te1 Mo1 Te1A F1 174.0(7) . . . . ? 
O4 Mo1 Te1A O5 -162.7(7) . . . . ? 
O2 Mo1 Te1A O5 80.4(6) . . . . ? 
O3 Mo1 Te1A O5 -37.1(8) 8_454 . . . ? 
O1 Mo1 Te1A O5 153.9(9) . . . . ? 
F1 Mo1 Te1A O5 -88.7(3) 3 . . . ? 
Te1 Mo1 Te1A O5 -132.3(6) . . . . ? 
 
_diffrn_measured_fraction_theta_max    0.985 
_diffrn_reflns_theta_full              27.12 
_diffrn_measured_fraction_theta_full   0.985 
_refine_diff_density_max    1.378 
_refine_diff_density_min   -1.693 
_refine_diff_density_rms    0.451 
